Tool and Die Making, Surface Treatment, and Repair by Laser-based Additive Processes

This paper explores the possibilities to use laser-based additive processes to make, surface treat and repair/remanufacture tools, dies and molds for cold working, hot working, and injection molding. The failures encountered in these applications are described. The materials used conventionally and in the laser additive processes are accounted for. The properties of the tools, dies and molds made by Laser-based Powder Bed Fusion (L-PBF) are as good as and in some cases better than the properties of those made in wrought materials. Shorter cycle time, reduced friction, smaller abrasive wear, and longer life cycle are some of the benefits of L‑PBF and Directed Energy Deposition with powder (DED-p) (or Laser Metal Deposition with powder, LMD‑p, or Laser Cladding, LC). L‑PBF leads to higher toolmaking costs and shorter toolmaking lead time. Based on a review of conducted investigations, this paper shows that it is possible to design and make tools, dies and molds for and by L‑PBF, surface functionalize them by DED-p (LMD‑p, LC), and repair/remanufacture them by DED-p (LMD‑p, LC). With efficient operational performance as the target for the whole tool life cycle, this combination of L‑PBF and DED-p (LMD‑p, LC) has the greatest potential for hot working and injection molding tools and the smallest for cold working tools (due to the current high L‑PBF and DED-p (LMD‑p, LC) costs).

Production tooling has also a large impact on the operational performance, costs, lead time, and quality. Cutting (material removal), cold working, hot working, and injection molding are some of the industrial tooling applications. Yet, cutting tools (material removal) are not covered in this review.
As displayed in Fig. 1, the tool material has a large influence on the tool life [1]. Tool material selection is based on (a) the required tool performance during the intended application and (b) the manufacturing of the tool. As far as the tool production is concerned, the tool material machinability, polishability, and heat treatment response are of great significance. Toughness, wear resistance, hot hardness, and resistance to softening are some of the important performance factors.
The failure mechanism encountered in cold working tools, e.g. stamping tools and dies, comprise abrasive and adhesive wear or mixed wear (caused by sliding contact), chipping at cutting edges and corners (fatigue), plastic deformation (exceeding the yield strength locally), cracking (fatigue), and galling (the same mechanism as in adhesive wear). The tool concept (tool material, hardness, surface roughness and treatment) is highly related to the workpiece material (sheet material grade, surface, and thickness). The tool concept for 1-mm thick hot-dip galvanized DP600 steel sheet differs therefore from that for 1-mm thick uncoated DP1000 steel sheet [2][3][4].
For hot-working tools, i.e. tools and dies in high pressure die casting, hot forging, hot stamping, or extrusion, thermal fatigue (heat checking), corrosion/erosion, cracking (total failure), and indentation are some of the failures that need to be avoided. Thermal fatigue is dependent upon thermal expansion coefficient (should be low), thermal conductivity (should be high), hot yield strength (should be high), temper resistance (a good resistance to softening at high temperature exposure), creep strength (should be high), and ductility. In other words, the tool should display resistance to deformation, softening, wear, impact loading and corrosion/erosion at the working temperature [5][6][7].
Some injection molds are likely to be exposed to corrosion, since the plastic materials can produce corrosive byproducts, e.g. PVC, and/or due to condensation caused by prolonged production stops, humid operating or storage conditions. In such cases, a stainless tool steel is required. Through-hardened molds are used if the production runs are long, abrasion from certain molding materials needs to be avoided, and/or the closure or injection pressures are high. Large molds and molds with low demands on wear resistance, however, can be made in pre-hardened steel. Good polishability and excellent surface finish are key requirements for many injection molds [8,9].
An efficient operational performance does not allow production stops and requires minimized tool maintenance time and costs. Tool repair and remanufacturing have several targets-preventive maintenance, refurbishment of the tool properties and performance, shortening of the production stops and reduction of the toolmaking lead time and costs.
The purpose of the present paper is to explore the possibilities of tool and die making, surface treatment and repair through laser-based additive processes, the industrial maturity of these processes and provide a brief future outlook in this regard. For tool and die making, the paper is focused on additive manufacturing (henceforth AM or 3D-printing) by Laser-based Powder Bed Fusion (L-PBF). For tool surface treatment and repair, Directed Energy Deposition with powder (DED-p) or Laser Metal Deposition with powder (LMDp) or Laser Cladding (LC) is at the focus. Fig. 2 displays a comparison of different metal AM methods with respect to part performance, cost, and lot size [10]. Production tools are normally made in single or few units and required to perform well in operation to avoid stops, minimize or eliminate rejections and maximize the production efficiency. L-PBF (PBF-L in Fig. 2) is, in other words, in a good position from these perspectives. The high L-PBF costs indicated in Fig. 2 are observed in many AM tooling related investigations (see, for instance, [11,12]).

Tool and Die Making
As mentioned above, the tool material has a large influence on the tool performance. Table 1 displays the properties of some of the conventionally made and used tool steels [13,14]. Table 2 shows the properties of the tools made by L-PBF in the displayed powder steels [15][16][17][18][19][20][21][22][23][24][25][26][27]. The powder steels  [10] in Table 2 are the most common steel powders used in tool and die making by L-PBF.
Design for AM, DfAM, can be divided into system design, part design, and process design (see also tool design in Fig. 1; [28]). Different selection criteria can be used to identify whether a redesign for AM would be beneficial [29]. The conducted studies confirm the importance of using the system, part, and process design approach and having efficient design as the selection criterion. The objective of efficient design is to improve the efficiency and performance of the tool in operation, i.e. shorter cycle time, avoidance of stops, minimization (or elimination) of the rejections, improved quality, maximization of the production efficiency etc. [11,25,[30][31][32][33][34][35][36].
Efficient design is of particular significance for the production tools in hot working and injection molding. The importance of process design and its close relationship to part and system design is illustrated in [36].
While the primary target is high efficiency and performance in operation, using generative design and topology and lattice structure optimization will also lead to lightweight design.
Using the efficient design, i.e. high efficiency and performance in operation, as the criterion, the conducted studies show that L-PBF, combined with conformal cooling and topology and lattice structure optimization, has its greatest potential in production tools for hot working and injection molding.  Table 2; [37]).
In HPDC of Al, the following failures should be avoided: a) heat checking due to thermal fatigue, b) erosion-hot mechanical wear, mainly due to the velocity of the melt,  Table 2; [37]) Cold-work steels The values are from [13].   [21], see also [22] Tool steel  [11] c) metal corrosion due to chemical interaction between Al & tool steel (e.g. high nickel), d) cracking due mechanical overloading of the die, e) soldering-molten alloy sticks to the die face, f) shrink porosity-bad temperature management leads to high scrap rate, and g) cracking from the cooling channel-high stresses in the mold based on wrong cooling channel design or stress corrosion.
While a)-d) are related to the tool (die or mold) steel, e)-g) are affected by the tool (die or mold) design, particularly the design of the cooling channels. Avoidance of a)-g) by proper material selection and DfAM resulted in the mold displayed in Fig. 3. The usage of this mold reduced the cycle time by at least 2.5% and the scrape rate to 3.4%. At the same time, the tool life was increased by at least 150% [37]. As mentioned above, the high L-PBF costs indicated in Fig. 2 are observed and reported in many investigations [10][11][12]27]. For the parts that require production tooling, the high L-PBF costs correspond to high tooling costs (see Fig. 4). For hot working and injection molding, the tools, dies, molds, cores, and inserts made by L-PBF cost more (see Fig. 4) but lead to lower total costs (the part costs), since such tools enable shorter cycle time, improved quality, and more.
For cold working (e.g. stamping), both the tooling and part costs are, however, higher (than the conventionally made tool and the part made in it) in case the tools are made by L-PBF [1,[10][11][12]27]. As a remedy to the late changes in product industrialization, the lead time reduction can justify the higher costs [1] (see Fig. 4).

Tool and Die Surface Treatment
Tool surface treatment is carried out to improve the tool's operational performance-wear or corrosion resistance, tribological properties, tool life, and more. Chemical Vapor Deposition (CVD), Physical Vapor Deposition (PVD), and plasma nitriding (PN) are some of the surface treatment methods used to improve the tool's operational performance.
The improvements that can be accomplished by such methods in cold working applications are described in, for instance, [2][3][4]38].
Laser-based additive processes have, however, enabled a hybridization-toolmaking through L-PBF in combination with the enhancement of the tool's operational performance, i.e. surface functionalization, through LMD-p (DEDp or LC).  Table 2) by L-PBF and left: hard-faced through LMD-p (DED-p or LC) with a Ni-based metallic matrix embedded with 60 wt% WC (NiCrSiB + 60 wt% WC), and right: coated by LMD-p with an aluminum-bronze (AlBz) layer [50].
For L-PBF, the layer thickness was 30 µm and the Yb-fiber laser effect 200W. For LMD-p (DED-p or LC), a high-power direct diode laser with a maximum output power of 10 kW was used. A linear-oscillating tribometer was used to study the sliding performance (reciprocating sliding, dry conditions, normal load of 31 N, frequency of 1 Hz, counterpart 100Cr6 cylinder with a hardness of ca 800HV, and test duration of 20 min). The abrasive wear resistance was evaluated in accordance with ASTM G65 [51].
Compared with the substrate made by L-PBF inDIN 1.2709, both surface-functionalized hybrids exhibited reduced friction coefficient. This coefficient was reduced by 25% with the Ni-based cladding. The hybrid hardfaced with NiCrSiB + 60 wt% WC displayed 45 times higher (better) wear resistance than the maraging steel substrate [51].

Tool and Die Repair and Remanufacture
A tool, die, or mold might be damaged or worn to an extent where it is no longer fit for purpose. Remanufacturing is defined as a process to "return a used product to at least its original performance with a warranty that is equivalent or better than that of the newly manufactured prod- Fig. 8: The part (product) production costs and the revenues versus the number of manufactured units. The figure concerns a part that requires production tools. Two options are displayed: the tool is made conventionally or by an AM inclusive process. The conventionally made tool is fully replaced with anew tooland thetoolmadebyL-PBFisrepaired/remanufactured byDED-p (LMD-p),astheprevioustoolisnotfitfor thepurposeanymoredueto damage uct" [52,53] (the product being the tool, die, or mold in the present paper). In case the part made by this tool is not to be phased out, repair, and remanufacture (and reuse) of the tool is of great significant for the operational efficiency. The die stands for 10-30% of the total costs of hot forged components [54], and it is essential to restart the production quickly and economically [52].
The failure mechanisms encountered in tools, dies, and molds in cold and hot working and injection molding are described in Sect. 1. Some of these failure mechanisms require repolishing (or surface cleaning by other methods), thin film surface treatment (CVD, PVD), or surface hardening by laser, nitriding, or boriding [54].
In other cases (e.g. cracking, heat checking, chipping, and/or abrasive wear), the damaged area needs to be removed by machining or scarfing after which it is repaired by Tungsten Inert Gas (TIG) welding, Gas Tungsten Arc Welding (GTAW), Electron Beam Welding, Plasma Transferred Arc Welding (PTAW), Cold Spray Method, Electro Spark Method, High-Velocity Oxyfuel (HVOF) thermal spraying, or laser based deposition (DED-p, LMD-p or LC in this paper) [55,56].
DED-p (LMD-p or LC) has a sufficiently high deposition rate, provides the best metallurgical properties, and has a short setup time but costs the most compared to the other mentioned methods [56].
Repair and remanufacture of hot forging, die casting, hot forming, extrusion and molding dies in wrought H13 by LC (LMD-p, DED-p) has been subject to several studies. LMD-p is considered as a replacement for flood welding, as hot forging dies in H13 are repaired and remanufactured [52]. Investigations have been carried out to study the LC of such dies with Co-based Wallex 40 and 50 [57,58], Stellite 21 [59,60], MetcoClad 21 [61], and H13 powder [62]. Repair by laser surfacing of die casting dies in maraging steel [63], and LC of wrought D2 by D2 powder [64] can also be mentioned as examples which display the high potential of DED-p (LMD-p, LC). Fig. 6 displays a hot forging die repaired/remanufactured by LMD-p. The nitrided H13 tool steel die with a hardness of approximately 60 HRC is used to produce components for forestry vehicles from a billet of boron-steel alloy (27Mn-CrB5-2). The die produces normally a maximum of 1300 parts before it is replaced. The purpose of the investigation was to study whether it was possible to repair a damaged die to achieve an equivalent life or better [61]. Fig. 6a shows the worn areas. After machining these areas, material was, as shown in Fig. 6b, added to the same areas through LMD-p. Fig. 6c depicts the fully repaired die after LMD-p and machining [61].
The selection of the material that was to be deposited was a key aspect. Therefore, a selection matrix was developed. This matrix included mechanical shock properties, thermal expansion compatibility, and wear characteristics. Forging tools are subjected to high impact forces during the manufacturing process. The material selected should therefore have suitable mechanical properties at operating temperature. The tooling operates at ≤ 500°C and a near uniform expansion (of the substrate and the added material) is therefore required to maintain tolerances and remain durable [61].
This scoring matrix was subsequently applied to a range of materials-MetcoClad 6, MetcoClad 21, Stainless Steel 420, Stainless Steel 316L, Inconel 625 and Inconel 718. Met-coClad 21, a CoCrMo alloy matrix containing dispersed hard carbides, was found to be the most suitable material [61].
To use the optimal LMD-p process parameters values, an investigation was carried out which included laser power (W), feed rate (mm/min), powder rate (g/min), pattern (linear or cross), and more [61].
Different LMD-p strategies were selected for the different worn areas. For, for instance, the cavity (area 2 in Fig. 6a), 2 layers, 0.7 mm per layer, 1 mm path overhang, and 1.2 mm stepover was the selected strategy [61].
The repaired/remanufactured die shown in Fig. 6c was able to produce 1400 forged parts (8% longer die life). No production issues were reported on the repaired die. Less die wear was observed on the MetcoClad 21 areas [61].
The tool remanufacture needs, however, to follow a methodology and be based on strategies that Fig. 6 and [52,59,61] exemplify. During the manufacturing engineering of a new product, it is now important to adopt a holistic view, which includes the tool lifecycle including the number of times the tool is (or can be) remanufactured. Efficient operational performance as the target for this whole tool lifecycle yields the largest potential for the laser additive processes, i.e. the combination of L-PBF and DEDp (LMD-p). This potential is the largest for hot forming and injection molding and the smallest for cold working due to the current high L-PBF and DED-p (LMD-p) costs. Fig. 8 displays the part (product) production costs and the revenues versus the number of manufactured units. The figure illustrates the cost and revenue factors that need to be considered for a part that requires production tools. Two options are displayed: the tool is made conventionally or by an AM inclusive process. The conventionally made tool is fully replaced with a new tool, as the previous tool is not fit for the purpose anymore due to damage. The tool made by L-PBF is repaired/remanufactured by DED-p (LMDp), as the previous tool is not fit for the purpose anymore due to damage.
Design for AM and L-PBF results in a tool that reduces the cycle time and therefore reduces the production costs. Breakeven is therefore reached faster with the tool made by L-PBF (see Fig. 8). The costs of conventional toolmaking and tool remanufacture by DED-p (LMD-p) and the revenue levels are of great significance and need to be identified/ estimated. Fig. 8 illustrates this significance, emphasizes the need of further cost studies, and the cost obstacle for a wider industrial spread of the laser additive processes in toolmaking. It also indicates the need of further research and development to improve the productivity and reduce the costs of L-PBF and DED-p (LMD-p) (see also Fig. 4).
According to non-peer-reviewed assessments, L-PBF has reached the highest industrialization index (i.e. widespread industrial use) and the highest technology maturity index (i.e. established full-scale produc-tion) compared to the other metal AM methods. DEDp is a step behind L-PBF with regard to both the industrialization index and the technology maturity [65]. L-PBF complies with high performance requirements, is suitable for small lot sizes and stands for high cost tolerances (compared to other metal AM methods). DEDp complies with medium to high performance requirements, is suitable for small to medium lot sizes and stands for medium cost tolerances [10] (see also Fig. 2). AM in tooling applications has the second highest manufacturing readiness level (AM in dental/medical applications has the highest) [66].
The size of the object than can be made by L-PBF is of great significance for many tooling applications. The maximum object size that can be made by L-PBF today is 600 × 600 × 600 mm 3 (although the largest height is 850 mm in one of the other current machines) [1]. Yet, many production tools, particularly (cold) stamping, press-hardening, and die casting tools, are larger than 600 × 600 × 600 mm 3 . L-PBF can be used to make tool, die, or mold inserts, which then are mounted in a core or shoe that is made by e.g. casting. Another option is to design the tool modularly and make each module or the modules with the greatest impact on operational efficiency by L-PBF. DED-p (LMD-p) can then be used for surface functionalization and tool, die or mold repair/remanufacturing. The mechanical properties of the tools, dies, and molds made by L-PFB are fully comparable and in some cases better than those of the tools, die, and molds made conventionally in the wrought materials (compare Table 2 with Table 1). The number of available powder materials for tooling applications is still very limited ( Table 2). More powder materials need to be developed for different tooling applications.

Conclusions
It is possible to design and make a tool (die or mold) for and by L-PBF, surface functionalize it by DED-p (LMD-p, LC), and repair/remanufacture it by DED-p (LMD-p, LC). With efficient operational performance as the target for the whole tool life cycle, this combination of L-PBF and DED-p (LMD-p, LC) has currently the greatest potential for hot working and injection molding tools and the smallest for cold working tools (due to the current high L-PBF and DED-p (LMD-p, LC) costs).
Funding. Open access funding provided by the Austrian Society for Metallurgy and Materials (ASMET).
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons licence, and indicate if changes were made. The images or other third party material in this article are included in the article's Creative Commons licence, unless indicated otherwise in a credit line to the material. If material is not included in the article's Creative Commons licence and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permis-sion directly from the copyright holder. To view a copy of this licence, visit http://creativecommons.org/licenses/by/4.0/.